Friction-stir welding of AA 2198 butt joints: mechanicalcharacterization of the process and of the weldsthrough DOE analysis
Ciro Bitondo & Umberto Prisco & Antonino Squilace &Pasquale Buonadonna & Gennaro Dionoro
Received: 9 June 2010 /Accepted: 28 July 2010 /Published online: 15 August 2010# Springer-Verlag London Limited 2010
Abstract In this study, rolled plates of AA 2198 T3aluminium alloy are friction-stir welded in butt config-uration varying two fundamental process parameters:rotational and welding speeds. Two sets of empiricalmodels based on regression analysis are developed. Thefirst one predicts the stationary values of the in-plane anddownwards forging welding forces in dependence of theprocess parameters under investigation. The second onepredicts the mechanical strength, in particular yield andtensile strength, of the friction-stir welded joints asfunction of the same parameters. For the developmentof the empirical models, two 32 full factorial designs areused: one having the stationary values of the weldingforces and the other having the yield and tensile strengthas observed responses, respectively. Statistical tools suchas analysis of variance, F tests, Mallows CP, coefficientof determination etc. are used to build and to validate thedeveloped models. By using the desirability functionapproach, the optimum process parameters to simulta-neously obtain maximum possible yield and tensilestrength are found within the investigated range. Thedeveloped models can be effectively used to predict thestationary forces and the mechanical proprieties of thejoints at 95% confidence level.
Keywords AA 2198 . Friction-stir welding (FSW) .
Rotational speed .Welding speed . FSW forces . Tensilestrength . Design of experiments, desirability function (DF)approach
Friction-stir welding (FSW) is a solid-state joiningprocess in which the material that is being welded doesnot reach the melting point, in contrast to the fusionwelding processes . Due to the interesting features ofFSW, lots of research activities have been carried out ondifferent materials (aluminium alloys first of all, but alsosteel, titanium, magnesium, copper, polymers etc.) and ondifferent weld geometries. In particular, FSW of AA 2198aluminium alloy has gained wide use in the fabrication oflightweight structures requiring a high strength-to-weightratio and good corrosion resistance .
In comparison with other welding techniques, FSWoffers advantages for low residual stresses, low distortionand high joint strength [2, 3]. Nevertheless, during thisprocess, the tool, with its rotational and welding speeds,exerts in-plane (horizontal) and downward (vertical)forging forces on the plates to be welded. These forces,joined to the thermal impact effect, may cause thedeformation of the fixture and of the welded plates, aswell as influence the tool wear. Hence, controlling theforce is mandatory for FSW and can have strongconsequences on the productivity and on the weld quality.Many significant benefits can be obtained keeping thewelding forces at a definite level: optimization of fixtur-ing, tool breakage prevention, tool life prediction, predic-tion of clamping forces, etc. Especially in robotic FSW,force controlling can be very helpful.
C. Bitondo :U. Prisco (*) :A. SquilaceDepartment of Materials and Production Engineering,University of Napoli Federico II,Piazzale Tecchio,Naples, Italye-mail: email@example.com
P. Buonadonna :G. DionoroDepartment of Mechanical Engineering, University of Cagliari,Piazza dArmi,Cagliari, Italy
Int J Adv Manuf Technol (2011) 53:505516DOI 10.1007/s00170-010-2879-9
However, to build an efficient control technique forFSW, a well-founded force prediction model needs to bedeveloped. The empirical model developed for the predic-tion of the welding forces can be further employed to getbetter insights into the mechanics of FSW, the correlationbetween the welding parameters and interdependencebetween the welding parameters and the weld quality.Development of FSW force models is not an easy taskconsidering that it was proved that the clamping forcecontains static nonlinearities with respect to the toolrotational speed, longitudinal speed, tool plunge depth andthe thermomechanical performance of the materials . Onthe other side, it is also essential to have a complete controlover the relevant process parameters to maximize the yieldand tensile strength on which the quality of a weldment isbased.
It has been proved by several researchers that efficientuse of statistical design of experimental techniques allowsdevelopment of an empirical methodology to incorporate ascientific approach in the FSW procedure . Indeed, thedesign of experiments was used in several papers toconduct experimental campaigns for exploring the interde-pendence of process parameters, and to develop empiricalmodels for the prediction of tensile strength of friction-stirwelded joints.
For instance, using the design of experiments concept,response surface method and the Hooke and Jeevesalgorithm, Elangovan et al.  developed a empiricalmodel to predict the tensile strength of friction-stir weldedAA 6061 aluminium alloy joints and optimized the FSWprocess parameters to attain maximum tensile strength. Themodel was developed by incorporating welding parametersand tool profiles and by using statistical tools such asdesign of experiments and regression analysis. Balasubra-manian  established an empirical relationships to predictthe FSW process parameters, in particular, tool rotationalspeed and welding speed, to fabricate defect free jointsfrom the known base metal properties (yield strength,ductility and hardness) of aluminium alloys. Lakshminar-ayanan et al. , based on a three factors three-level centralcomposite design with full replications, developed aresponse surface methodology to predict the tensile strengthof friction-stir welded AA7039 aluminium alloy.
However, to the present authors' knowledge, sparsework has been carried out on prediction of both weldingforces and mechanical proprieties of joints in FSW.
Therefore, in this investigation an attempt is made todevelop empirical models for the prediction of weldingforces and mechanical strength (yield and tensile) offriction-stir welded joints. In addition, it is tried tooptimize the FSW process parameters to attain maximummechanical strength of friction-stir welded joints using thedesirability function approach.
2 Experimental work
Rolled plates of 3.2 mm thickness AA 2198 T3 aluminiumalloy were cut into the required size (200100 mm) bypower hacksaw cutting. The chemical composition andmain mechanical properties of base alloy are listed inTables 1 and 2.
The obtained plates were used to fabricate FSW joints inbutt configuration (welds are 200 mm long), see Fig. 1a.The direction of welding was parallel to the rollingdirection. Non-consumable tools, made of Cr-Mo steel,were used to fabricate the joints. Tool geometry ischaracterised by a shoulder radius of 12 mm and by anunthreaded cylindrical pin of 4 mm in diameter and 3 mmlong. The forging action of the tool shoulder was enhancedby a forwards tool tilt angle of 2. The plates were butt-welded using a five axes DMG CNC universal millingmachine with a 0600600 (x/y/z) workspace. Themachine was instrumented with a Kistler three-axis dynam-ic dynamometer for in-plane, Fx, and downwards forging,Fz, welding forces recording. For the force signal acquisi-tion, the sampling rate was set at 10 Hz.
In all the experimental campaign, the welding processwas divided in the following phases:
a) initial phase, during which the pin, moving along the z-axis, reaches the plates surfaces and penetrates into thematerial up to the shoulder;
b) plunging phase, during which the tool shoulder reachesthe surface and is plunged into the joint line until theshoulder deepens 0.1 mm underneath the top surface so
Table 1 Chemical composition (wt.%) of base AA 2198 aluminium alloy
Si (%) Fe (%) Cu (%) Mn (%) Mg (%) Cr (%) Zn (%) Zr (%) Li (%) Ag (%)
Min 2.90 0.25 0.04 0.80 0.10
Max 0.08 0.10 3.50 0.50 0.80 0.05 0.35 0.18 1.10 0.50
Table 2 Mechanical properties of AA 2198 T3 perpendicular to therolling direction
UTS (MPa) YS (MPa) E (GPa) Elongation (%)
370 275 15
506 Int J Adv Manuf Technol (2011) 53:505516
attaining the right frictional contact (throughout thisand the previous phases, the feed rate of the tool alongthe vertical axis was set at 5 mm/min and keptconstantly at this value);
c) dwelling phase, lasting 4 s, during which the tool,rotating on the same position, softens the materialthrough frictional heating;
d) welding phase, during which the tool is advanced alongthe joint line and the weld is realized.
To study the dependence of the stationary welding forces(see below) on process parameters a two factors, three levels,design matrix, with the central point replicated four times toestimate variance due to experimental or random variability isadopted. A 32 full factorial design results. This design required
9+3 (replications)=12 runs, including the replicated centralpoint. The treatment variables (factors) subjects of this studyare the rotational, N (rpm), and welding speed, V (mm/min).Each factor has three levels. The observed responses are thestationary values of the in-plane and forging forces reachedduring the welding steady state. Trial experiments werepreliminarily conducted to determine the working range ofthe above factors. Feasible limits of the parameters werechosen in such a way that the friction-stir welded jointsresulted free from any visible external defects. Macrographsof the welds showed a typical FSW macrostructure consistingof a stir zone (nugget), thermo-mechanically affected zone andheat-affected zone. Figure 1c reports as example the macro-graph of the joint #1 of Table 6; the nugget and the onionrings can be easily identified. The chosen experimental designlevels of the independent variables are: 500, 700 and 900 rpmfor N; 150, 225 and 300 mm/min for V. Figure 2 reports thetreatment combination of the above described 32 factorialdesign hereinafter called the FSW force design.
To evaluate the mechanical proprieties of the butt joints,after the welding process, the joints were sliced, as shown inFig. 3a, using a power hacksaw and then machined torequired dimensions as shown in Fig. 3b. Three tensilespecimens were fabricated for each joint following theAmerican Society for Testing of Materials (ASTM E8M-04) standards. Hence 123=36 specimens were obtained.The tensile tests were carried out at a strain rate of 104 on aMTS servo-hydraulic testing machine. For each tensile test,the yield strength at 0.2% offset, from now on simply YS(MPa), and the tensile strength (UTS (MPa)) of the weldswere determined.
All welds and tests were executed in a randomized order toexclude the disturbing effects of environmental conditions.
Although the specimens were obtained from differentpositions on the weld, in the analysis of weld mechanicalproprieties, this variable is not considered. Indeed, by means ofa Nec TH 7800 thermo camera it was checked that heat fluxreached a steady-state condition during the FSWas soon as thewelding phase starts. In particular, it was checked that the
Rotational speed, N [RPM]
m / m
Fig. 2 Treatment combination in the 32 FSW force design
Strain [%]0 2 4 6 8 10 12 14
Fig. 1 a Configurations of the workpiece, tool and fixture tableduring the FSW; b macro-photography of the FSW joint #1 ofTable 6; c engineering stressstrain curve for the specimen # 1 ofTable 6
Int J Adv Manuf Technol (2011) 53:505516 507
different points along the weld length experience similartemperature history. As a consequence, considering that theamount of the heat conducted into the workpiece dictates thequality and micro-structure of the weld, as well as the residualstress and its mechanical strength, it is possible to conclude thatthe weld presents the same mechanical proprieties along itslength. Subsequently, the 36 tensile tests constitute a 32 fullfactorial design with several repeated points, as it is specifiedin the followings. In particular, the independent variables areagain N and V, characterized by the same previous threedesign levels, while the observed responses are now YS andUTS of the welds. The treatments combination of this designderives from the one reported in Fig. 2 repeated three timesbeing three the specimens extracted for each combination ofrotational and welding speed. As a result, the central point isrepeated 12 times, i.e. 43 (the four-times repeated centralpoint of the FSW force design in Fig. 2 times the threeextracted specimens). From now on, it will be referred to thisdesign as the weld strength design.
3.1 Empirical models of the FSW stationary forces
The in-plane and downwards forging forces detected duringthe welding process have a diagram showing identical
features for all the different welding conditions. In Fig. 4,the principal features of the FSW forces-time plot moni-tored during the run 4, according to the numbering inTable 3 (N=700 rpm, V=150 mm/min), are shown. Figure 4indicates that the vertical force, Fz, rapidly rises to a firstpeak value during the insertion of the pin into the material.The pin insertion proceeds with some instability phenom-ena, revealed by some other peaks followings this first one,and caused by the material being still cold. Straightafterwards, the frictional heat generated by the pin softensthe alloy so that the vertical force undergoes a relaxationfrom the previous peaks. In the subsequent phase, inparticular when the shoulder reaches the material and startsplunging into the surface of the top sheet, the vertical forceagain increases due to the added frictional work. During thedwelling phase, this steep increase of Fz is once againfollowed by a reduction of the vertical force due to theplasticization induced into the material by the friction heat.At the beginning of the welding phase, Fz starts rising veryrapidly. When the FSW process attains the steady state, thevertical force reaches a stationary value, which is thehighest value achieved by Fz in all the different weldingconditions investigated. Finally, the vertical force plungesdown to zero as the shoulder looses contact with the surfaceand the pin is extracted from the material. By increasing thetool rotational speed, the height of the different peakdecreases. However, Fz gets a stationary value for all theinvestigated welding conditions; this value is characteristicof the adopted FSW process parameters. On the contrary,the horizontal force, Fx, simply oscillates around zero up tothe beginning of the welding phase, when it suddenlyreaches a stationary value that keeps until the tool pinextraction. This value is also characteristic of the adopt...